# Semiconductor Processing: Crystal Growth · 2014-10-27 · A brief introduction to crystal...

date post

12-Mar-2020Category

## Documents

view

1download

0

Embed Size (px)

### Transcript of Semiconductor Processing: Crystal Growth · 2014-10-27 · A brief introduction to crystal...

Semiconductor Processing:Crystal Growth

Professor Benjamín AlemánDepartment of PhysicsUniversity of Oregon

How do we make these useful and curious structures?

2 µm

5 µm

1 μm

Planar Processing with Semiconductors (Silicon):Course Map

• Crystal growth (semiconductors)• Wafer characteristics• Wafer doping• Defects and impurities• (SiO2 growth)

• (SiO2 growth)• Masked doping• Lithography• Vacuum Systems• Thin Films: CVD, MBE,

PVD, ALD• Implantation• Wet and Dry Etching• Integration

Why are semiconductors useful?

II III IV V VI

Types of Semiconductors:

• Si: Elemental• GaAs: III-V Binary Compound• ZnSe, CdTe: II-VI Binary• Organic

Why is Silicon an important semiconductor and why is it so popular in planar processing?

• 26% by mass of Earth’s crust

• Over 90% of Earth’s crust is silicate materials.

Silicon is abundant

Ge

A brief introduction to crystal structure

Crystal Structure = Lattice + Basis

A lattice is defined by a set of fundamental translation vectors ��, ��, ��, such that the atomic arrangement looks the same from the perspective of both � and ��, where

�� = � + ���� + ���� + ����and ��, ��, �� are arbitrary integers.

The basis

Lattice?

Basis

Cubic lattices

Salt is FCC with basis containing one Na and one Cl.

Diamond is FCC with two identical basis atoms:

All group IV elements can crystallize into diamond, including C and Si.

Index system for crystal planesCrystal planes are identified using Miller indices in the following way:

1. Find the intersection of the axes in terms the basis of the fundamental translation vectors ��, ��, ��.

2. Take the reciprocal and reduce to three integers having the same ratio, usually the smallest three integers. The result is enclosed in parentheses (ℎ��) and called the index of the plane. Negative integers are denoted with bars (ℎ���).

Also, planes equivalent by symmetry are denoted with braces {ℎ��}.

• The set of cube faces is {100}.

The indices [���] of a direction in a crystal are the set of the smallest integers that have the ratio of the components of a vector in the desired direction.

• The ��axis is the [100] direction, the −�� axis is the [01�0] direction.

• NB: In cubic crystals, the direction [ℎ��] is perpendicular to the plane (ℎ��) having the same indices.

Index system for crystal planes

Plane intercepts the vectors ��, ��, �� axes at 3��, 2��, 2��. Reciprocals of

these numbers are �

�,

�

�,

�

�. Small integers having the same ratio are 2, 3, 3,

thus indices of the plane are (233).

Examples of indexed crystal planes

Si (100)Si (111)

Crystal Growth: Silicon and Gallium Arsenide

Advantages of Si Advantages of GaAs

• Cheaper• More stable and less defects,

better for VLSI• Bigger wafers• SiO2• Pure element, easier to make• Higher hole mobility (for CMOS)

• Higher electron mobility• Higher saturation velocity• Good for MW electronics (250GHz)• Direct Band Gap: emits and absorbs

efficiently; for LEDs, Lasers, and PVs• Can make AlxGa1-xAs which allow

HEMTs.

• How we make single-crystal Si and GaAs?• How we shape into wafers?• Characteristics of wafers?

Manufacture of single-crystal Silicon requires high purity raw Silicon, made by the Siemens Process

Quarzite Carbon

98% pure MGS, which is then pulverized

Forms trichlorsilane (boils at 32 C), which is then distilled for hydrogen reduction

Produces very pure polycrystalline EGS on a heated Si rod in chamber. Impurity range is in parts-per-billion (ppb).

+

The Czochralski (CZ) technique: the crystal puller

The CZ technique in pictures

1412° CDopants(e.g. B)

[111] or [100] Si ingots are 200 kg in mass and 300 mm in diameter

Molten Si freezes onto Si seed.

Wafer size projections

?

The bigger, the cheaper?

How is do we dope Silicon?

Doping profiles of Silicon ingots

The concentration of dopant in liquid and solid phases of Si is not the same and changes during growth.

The equilibrium segregation coefficient:

�� = C�/C�

Equilibrium concentrations

�� < 1 means dopants are rejected by solid Si into the melt, so concentration in melt increases during growth. Also, if �� increase, then �� will too.

How does an increasing/decreasing dopant concentration in the liquid (��) affect the dopant

concentration (��) in a growing Si crystal?

Doping distribution of Silicon ingots during growth

• Example�/��

Effective Segregation Coefficient

During crystal growth, the dopant can accumulate near the liquid-solid interface and cause a dopant concentration gradient (�� < 1):

How can we model the system to account for the stagnant layer?

Mass transport by diffusion and drift